Microstructure and mechanical properties of short-carbon ... Microstructure and mechanical...
Embed Size (px)
Transcript of Microstructure and mechanical properties of short-carbon ... Microstructure and mechanical...
Journal of Advanced Ceramics 2020, 9(6): 716–725 ISSN 2226-4108 https://doi.org/10.1007/s40145-020-0408-3 CN 10-1154/TQ
Microstructure and mechanical properties of
Guangqi HEa,b, Rongxiu GUOa, Meishuan LIb, Yang YANGb,c, Linshan WANGd, Yuhai QIANb, Jun ZUOb,
Jingjun XUb,*, Changsheng LIUa,*
aSchool of Materials Science and Engineering, Northeastern University, Shenyang 110819, China bShenyang National Laboratory for Materials Science, Institute of Metal Research,
Chinese Academy of Sciences, Shenyang 110016, China cSchool of Materials Science and Engineering, University of Science and Technology of China,
Shenyang 110016, China dCollege of Science, Northeastern University, Shenyang 110819, China
Received: March 30, 2020; Revised: July 8, 2020; Accepted: July 13, 2020 © The Author(s) 2020.
Abstract: Short-carbon-fibers (Csf) reinforced Ti3SiC2 matrix composites (Csf/Ti3SiC2, the Csf content was 0 vol%, 2 vol%, 5 vol%, and 10 vol%) were fabricated by spark plasma sintering (SPS) using Ti3SiC2 powders and Csf as starting materials at 1300 ℃. The effects of Csf addition on the phase compositions, microstructures, and mechanical properties (including hardness, flexural strength (σf), and KIC) of Csf/Ti3SiC2 composites were investigated. The Csf, with bi-layered transition layers, i.e., TiC and SiC layers, were homogeneously distributed in the as-prepared Csf/Ti3SiC2 composites. With the increase of Csf content, the KIC of Csf/Ti3SiC2 composites increased, but the σf decreased, and the Vickers hardness decreased initially and then increased steadily when the Csf content was higher than 2 vol%. These changed performances (hardness, σf, and KIC) could be attributed to the introduction of Csf and the formation of stronger interfacial phases. Keywords: Ti3SiC2; short-carbon-fibers (Csf); spark plasma sintering (SPS); microstructure; mechanical
Ti3SiC2, a typical member of the MAX phase family, is a ternary layered compound. It has attracted extensive attention for its unique combination of metals and ceramic
* Corresponding authors. E-mail: J. Xu, firstname.lastname@example.org;
C. Liu, email@example.com
properties, such as low density, easy machinability, high melting point, high tensile strength and damage tolerance, excellent thermal shock resistance, good chemical stability, and oxidation resistance (< 900 ℃) [1–7]. Therefore, Ti3SiC2 is a potential structural material for applications in environments of high temperature, oxidation, corrosion, and wear, etc. [1,2,7,8]. However, low fracture toughness (KIC) and hardness limit its practical applications. The introduction of the second phase as reinforcement into Ti3SiC2 has been proved to
J Adv Ceram 2020, 9(6): 716–725 717
be an effective approach to overcome these disadvantages. For example, numerous reinforcements, including TiB2 , SiC , c-BN , TiC , Al2O3 , and ZrO2 , have been introduced to improve the mechanical properties of Ti3SiC2. Commonly, the addition of ceramic particles can improve Vickers hardness and flexural strength (σf) of Ti3SiC2 matrix composites. For example, Górny et al.  reported that the addition of TiB2 could effectively improve the Vickers hardness and elastic modulus of Ti3SiC2. Tian et al.  prepared Ti3SiC2–TiC composites and found that the Vickers hardness of the composites increased with increasing TiC content up to 90 vol%, and the σf was enhanced by 64% when the content of TiC was 50 vol%. Wang et al.  fabricated Ti3SiC2–xAl2O3 (x = 0–20 vol%) composites by spark plasma sintering (SPS), and found that Ti3SiC2–20 vol% Al2O3 exhibited the highest Vickers hardness, but other mechanical properties deteriorated because of the aggregation of Al2O3 in the composite. On the other hand, the toughness of Ti3SiC2 matrix composites has hardly ever been strengthened due to intrinsic brittleness of these ceramic phases.
Carbon fibers, with numerous attractively compre- hensive properties, such as low density, high strength and modulus, excellent chemical inertness, and small thermal expansion coefficient, are considered to be the most promising reinforcing phase for many structural ceramics [15–17]. Especially, short-carbon-fibers (Csf) have been applied extensively in the preparation of ceramic matrix composites by using SPS or hot-pressing (HP), due to their low cost, easy addition, and chemical inert at high temperatures. Csf reinforced ceramic matrix composites usually possess relatively higher KIC. For example, Wang et al.  fabricated Csf (up to 1 wt%) reinforced B4C composites, and found that the composites had higher KIC compared with monolithic B4C due to the occurrence of crack deflection and bridging resulting from interface debonding between fiber and matrix. Similarly, when Csf was introduced in ZrB2–SiC composites, the toughness of the composites was significantly improved, resulting from fiber debonding, pulling-out, and bridging as well as crack deflection . Unfortunately, the literature on Csf reinforced Ti3SiC2 composites is relatively scarce, only Lagos et al.  prepared Ti3SiC2–Cf composites by SPS, and the processing, microstructure, and thermo-mechanical properties (thermal expansion coefficient and thermal
conductivity) were investigated, but the mechanical properties of Csf reinforced Ti3SiC2 composites are not available.
In this work, Csf/Ti3SiC2 composites (the content of Csf was 0 vol%, 2 vol%, 5 vol%, and 10 vol%) were fabricated by using the SPS technique. The interfacial microstructure between Csf and Ti3SiC2 matrix and the effects of Csf introduction on room-temperature mechanical properties of Csf/Ti3SiC2 composites were systematically investigated, and the role of Csf addition played in reinforcement effect was also discussed.
2. 1 Material preparation
Ti3SiC2 powders (Forsman Technology Co., Beijing, China) and Csf (ZLXC, Co., Cangzhou, China) were used as raw materials. The purity and mean particle size of Ti3SiC2 powders was 98% and 3–5 m, respectively, and the main impurity was Al2O3. The length and diameter of Csf were 3 mm and 7 µm, respectively. Four Csf/Ti3SiC2 composites with Csf volume fractions of 0 vol%, 2 vol%, 5 vol%, and 10 vol% were fabricated using SPS (SPS-30T-15-3, Chenhua (Shanghai) Technology Co., Ltd., Shanghai, China). For convenience of the following description, the composites were denoted as 2, 5, and 10 Csf/Ti3SiC2, accordingly.
The preparation process of Csf/Ti3SiC2 composites is schematically illustrated in Fig. 1. Firstly, Csf was dispersed into deionized water with carboxymethyl cellulose sodium (CMC–Na) as the dispersant . The mass ratio of CMC–Na and Csf was 1:3. Then, Ti3SiC2 powders were added into the as-prepared solution. After stirring with a magnetic stirrer, the slurry of Ti3SiC2 powders and Csf was obtained. Dried in an oven, the mixed material was packed into cylindrical graphite die. Following, a green body with a diameter of ϕ 40 mm was obtained by cold pressing under a load of 20 MPa. Subsequently, the sintering was conducted in the SPS facility. After the vacuum of 10 Pa in the sintering chamber was acquired, the green body was heated to 1300 ℃, under the constant pressure of 40 MPa soaked for 8 min and the heating rate of 50 ℃/min. The as-prepared composite was then cooled to room temperature in the sintering chamber. All composites were fabricated under such identical SPS conditions.
718 J Adv Ceram 2020, 9(6): 716–725
Fig. 1 Schematic illustrations of the preparation process of Csf/Ti3SiC2 composites using SPS.
2. 2 Characterizations of composition and
microstructure of the composites
The actual densities of Csf/Ti3SiC2 composites were determined by Archimedes’ method. The phase compositions were performed on a D/max-2400 X-ray diffractometer (XRD) (Rigaku, Tokyo, Japan) with a Cu Kα radiation (λ = 0.1542 nm). The tube voltage was 50 kV, and the current was 100 mA. The 2θ range was (8°–80°) with a count time of 1 s per 0.02 (°)/step. The microstructure, cross-section morphologies, and fracture surfaces of the composites were performed by scanning electron microscope (SEM, Oberkochen, Germany, EHT = 20.00 kV) with energy dispersive spectrometer (EDS, Oxford Instruments, UK) in a vacuum.
2. 3 Determinations of mechanical properties
For mechanical tests, the samples were cut into a series of bars from the as-prepared composites by electrical discharge machining. Before testing, the surfaces of all samples were sanded to 2000 SiC sandpaper, polished to a mirror surface with 1.0 mm diamond paste, then ultrasonically cleaned in ethanol and distilled water, and finally dried.
The Vickers hardness test was carried out using Vickers indenter (432SVD, WOLPERT, USA) at a load of 9.8 N for 15 s. The parallel operations were conducted nine times, and finally, the mean value was obtained for each sample.
All mechanical performance tests were conducted on a universal testing machine (SANS, CMT4204,
Shenzhen, China). Three samples in each group were used for the σf and KIC measurement.
Three-point bending tests were employed to determine σf. The dimensions of rectangular samples were 3 mm ×